Share this document with a friend

7

Transcript

88-02- 28 -

UDC 621 . 791 . 9 . 052 . 2 : 539 . 415

Tensile Shear Strength of Laser Welded Lap Joints Yasunobu MIYAZAKI*1 Seiji FURUSAKO*2

Abstract

The dependency of fracture position and maximum load of laser welded lap joints

on the weld-bead length and width was clarified through tensile shear test of joints,

and a mechanical prediction model for the test results was developed. Joints showed

the strength proportional to base metal tensile strength, which have the weld length

over 60% of specimen width or the weld width of 2 times of sheet thickness. The

developed model, which considers a joint dividing it into the base metal under uniaxial

tensile stress, a portion R under stretch bending and the weld metal under shear

stress, proved capable of qualitatively predicting the fracture behavior of laser welded

lap joints of mild steel sheets at tensile shear test.

1. Introduction Resistance spot welding has long been employed as a principal

welding method for assembling automobile bodies, but some carmakers, mainly in Europe, recently use laser welding in place of resistance spot welding1,2). Laser welding is a non-contact welding method and capable of joining materials by one-side access. While the European carmakers reportedly find laser welding economically advantageous because the electrode wear of spot welding can be avoided, they do not seem to fully enjoy the benefits of laser welding such as easy connection of hydro-forming parts and other closed- section components and higher joint strength due to continuous welding. A reason for this is presumably that the application of laser welding is generally limited to those portions where spot welding can be used as a backup in the case of a trouble with laser welding, and another is that the advantages of continuous welding by laser are not very clear.

Furthermore, unlike spot-welding joints, laser-welding joints are not axisymmetric, and many variables such as weld length, bead width and welding direction affect the strength of a joint of laser welding, and for this reason, the withstand load of a laser-welding joint has not been clear. In view of this, the authors already proposed a method for estimating the strength of laser welded lap joints3). In the present study, the authors partially reviewed the regression analysis employed for the estimation, and attempted to express the relationship between the size of a weld bead and joint strength in a simplified manner.

2. Shear Strength of Laser Welded Lap Joints 2.1 Experimental procedure

An experimental examination was conducted on the tensile shear strength of laser welded lap joints. Table 1 shows the mechanical properties of the steel sheets employed in this study; the sheet thickness was 1 mm and their tensile strength varied from 300 to 800 MPa. Fig. 1 schematically shows the test piece for the tensile shear test. An Nd-YAG laser having a work-piece power of 1.6 kW was used for welding the test pieces. To examine the effects of the bead size on joint strength, the weld length and width were changed by welding across the whole width of the test pieces or partially (weld lengths L

b of 50 and 30 mm, respectively) and setting the welding

speed at 1.6 and 0.7 m/min (weld widths W b of 0.85 and 2 mm,

respectively). Table 2 summarizes the welding conditions.

*1 Steel Research Laboratories *2 Nagoya R&D Lab.

Table 1 Mechanical properties of steels used

Steel

A

B

C

D

Thickness

(mm)

1

1

1

1

YP

(MPa)

142

339

392

435

TS

(MPa)

301

472

629

794

Elongation

- 29 -

The tensile shear test was conducted at room temperature and at a constant tension speed of 10 mm/min, and the maximum withstand load of each weld joint was measured. To examine the deformation of the test pieces, some of them were loaded to withstand load, the load was removed before failure, and the deformation around the weld joint was recorded through sectional observation. 2.2 Tensile test results

In the tensile shear test of laser welded lap joints, fracture occurred at the base metal (BM), weld metal (WM) or portion adjacent to the weld joint (herein referred to as the portion R). Fig. 2 shows the photographs of test pieces after fracture at different portions and schematic illustrations of the fracture portions, and Fig. 3 shows the relationship between the maximum load that the lap joints withstood before fracture (hereinafter written as the joint strength) and the strength of the base metal. The dotted line of the graph shows the product of the tensile strength (TS) and sectional area of the base metal, namely the maximum withstand load of a joint in the case of fracture at the base metal (hereinafter written as the base-metal strength insofar as it is not confused with the tensile strength of the base metal).

As Fig. 3 shows, when the weld width was 2.0 mm and the weld length was 50 mm across the whole width of the test piece, the fracture occurred at the base metal or portion R, and the joint strength was the same as the base-metal strength. In contrast, when the weld width was 0.85 mm and the weld length was 50 mm, the weld metal failed except for the test pieces of Steel A, the joint strength increased as the base-metal strength increased, and the joint strength did not decrease significantly below the base-metal strength. On the other hand, the test pieces of Steel A failed at the portion R, and the joint strength was equal to the base-metal strength.

When the bead width was 2.0 mm and its length was 30 mm, all the test pieces failed at portion R, and the joint strength increased as the base-metal strength increased. In contrast, when the bead width was 0.85 mm and the length was 30 mm, the weld metal failed except for the test pieces of Steel A, but different from the cases where the

weld length was 50 mm, the joint strength was nearly the same, not depending on the base-metal strength. The test pieces of Steel A failed at the portion R even though the bead width was as small as 0.85 mm. 2.3 Deformation under load

Part (a) of Fig. 4 shows a sectional view of a test piece deformed under a tensile load; the base metal is Steel A and the weld joint is 2.0 mm wide and 50 mm long. Before application of a tensile load, the thickness center planes of the two sheets were out of alignment from each other, but under a tensile load, the test piece underwent a torque about the weld metal. When the tensile load increased, the deformation increased such that the thickness center planes of the two sheets aligned with each other. On the other hand, the test piece shown in the lower frame of part (b) of Fig. 4, which had a weld width of 0.85 mm, failed at the weld metal before the thickness center planes of the two sheets were aligned with each other.

Fig. 1 Schematic diagram of laser lap joint for tensile shear test

Table 2 Welding conditions for tensile test specimens

Beam source

Focal position

Weld length L b (mm)

2kW Nd-YAG laser

0.7, 1.6

2, 0.85

30, 50

Fig. 2 Fracture mode of laser lap joint in tensile shear test

Fig. 3 Dependency of laser lap joint strength on tensile strength of steel

NIPPON STEEL TECHNICAL REPORT No. 95 January 2007

- 30 -

3. Mechanical Model of Stresses in Laser Welded Lap Joints under Tensile Shear Test Although it is possible to experimentally determine the strength

of joints having different weld lengths, weld widths and sheet widths, it is a tiresome and time-consuming business. In view of this, an attempt was made to construct a model to estimate the strength of a weld joint in consideration of the stress imposed on the joint by a tensile load. 3.1 Modeling of stresses at different portions of joint

The deformation of a joint shown in Fig. 4 (a) indicates that such a deformation can be studied dividing a joint under a tensile load into three portions: the weld metal, portion R and base metal shown in Fig. 5. The stress in each of these portions under a certain load can be estimated by studying it in a simple manner separated from that in the other portions. 3.1.1 Stress imposed on base metal

When the bead length and width are sufficiently large and the fracture occurs at a position away from the weld metal as shown in Fig. 2 (a), the base metal is considered to be under a uniaxial tensile stress just like a single-sheet test piece at tensile test. Under an outside force T, therefore, the stress imposed on the base metalσ

B can be

estimated using the following equation:

σB = T Ws ⋅ t (1)

where, W s is the width of the specimen, and t is its thickness.

We introduce a dimensionless parameterβ according to Equa- tion (2), which is the ratio between the stress on the base metalσ

B

:

β = σ B / TSBM (2)

Here, the value ofβ changes from 0 to 1, and the joint fails at the base metal when the stress increases toβ = 1.0.

Eliminating the stress σ B from Equations (1) and (2), the outside

force T can be expressed as follows using the dimensionless parameter β , which expresses the magnitude of the load:

T = β ⋅ TSBM ⋅ Ws ⋅ t (3)

3.1.2 Stress imposed on portion R Here, let us simplify the portion R as being in a tension bending

condition as shown in Fig. 6. This seems to be an adequate approximation as far as the center of the portion R is concerned,

Fig. 4 Deformation of lap joint under tensile shear load and configuration after fracture, through cross-section of joint

Fig. 5 Simplified model of joint and geometric demand for configu- ration

Fig. 6 Definition of parameters at portion R

NIPPON STEEL TECHNICAL REPORT No. 95 January 2007

- 31 -

excluding its interfaces with the base metal and weld metal. With respect to the case shown in the upper frame of Fig. 4 (b) where a joint fails at a position in the curved portion (portion R) a little away from the weld metal, this simplification would be adequate for a model for predicting the position of fracture.

Following a common analysis method of bending deformation, we suppose a neutral plane where there is no tension or compression: there is a compressive stress on the inner side of it and a tensile stress on the outer side.

Letting the curvature radius of the neutral plane be R e , the

circumferential strainε(r) at a plane away from the curvature center by a distance r is given as follows:

ε r = r ⋅ θ − Re ⋅ θ

Re ⋅ θ

= r − Re

Re

(4)

In addition, the relationship between the curvature radius R i of the

inner surface of the portion R, the curvature radius R e of the neutral

plane and the distance a between the neutral plane and the thickness center shown in Fig. 6 is given by the following equation:

Re = Ri + t / 2 − a (5)

Furthermore, using a relational expression frequently applied to the relationship between stress and strain, the relationship between the circumferential stressσ (r) and strainε (r) is given as follows:

σ r = F ⋅ εn r (6)

where, F is the modulus of longitudinal elasticity, or Young’s modulus, and n is a work hardening coefficient.

Based on the above and supposing that the integration of the circumferential stress in the portion R is equal to the tensile load T, the following equation can be obtained.

T = Lb σ r dr Ri

Ri + t

(7)

where, L b is the weld length. This integration is easily carried out by

using Equations (4), (5) and (6), and the following equation is obtained:

T = Lb ⋅ F n + 1

1 Re

(8)

Here, the thickness t was assumed not to change under the deformation.

The value ofσ (r) becomes largest at the outer surface, and the largest valueσ

R is given as follows:

σ R = F ⋅ t / 2 + a Ri + t / 2 − a

n

(9)

A joint is expected to fail at the portion R when the value ofσ R reaches

the tensile strength TS R determined by the material quality of the portion

R. 3.1.3 Stress imposed on weld metal

In the case where a joint fails at the weld metal, as shown in Fig. 4 (b), the weld metal fails by shear fracture without significant deformation. The average shear stressτimposed on the weld metal under a tensile load T is expressed by Equation (10) below.

τ = T cos θ Lb ⋅ Wb

(10)

Lb ⋅ Wb cos θ (11)

where, θis the tilt angle of the weld joint resulting from the tensile load shown in Fig. 7, and W

b is the weld width as measured between

the two sheets. The dimensionless parameterβ , which expresses the magnitude of the load in Equation (3), was used for the modification from Equation (10) to Equation (11).

While shear stress is estimated at 1 / 3 times tensile strength, tensile strength TS is known to be in good correlation with Vickers hardness Hv, and when stress is expressed in terms of MPa, the relationship between these two is expressed as TS = Hv/3× 9.8. Therefore, when the hardness of weld metal Hv

WM is given, it is

possible to estimate the maximum shear stress τ max

that the weld metal can withstand by the following equation:

τ max = TSWM / 3

(12)

A joint is expected to fail by shear fracture of weld metal when the shear stressτgiven by Equation (11) becomes equal to the maximum shear stressτ

max given by Equation (12).

To estimate the shear stressτ imposed on weld metal based on Equation (11), however, it is necessary to know the tilt angleθ . 3.1.4 Relationship between tensile load and tilt angle of test piece

Let us suppose that, in Fig. 5, the weld metal, portion R and base metal connect to each other smoothly, that is, the boundary lines between the portion R and base metal are perpendicular to the direction of the tensile load. Here, it is easy to calculate the vector a from the weld center C to the thickness center X on the boundary line between the portion R and base metal and the vector b from the curvature center O of the portion R to the point X. These two vectors are perpendicular to each other when the deformation is well advanced and the thickness centers of the two sheets are aligned with each other. This geometrical demand is expressed as follows using the vector c from the curvature center O to the weld center C:

a ⋅ b = b − c ⋅ b

= Ri + t 2 ⋅ 1 − cos θ ⋅ Ri + t

2 + Wb

= 0

Since R i t / 2 is positive, the following equation is obtained:

Fig. 7 Stress state at each part of joint

NIPPON STEEL TECHNICAL REPORT No. 95 January 2007

- 32 -

2 − Wb

1 − cos θ (13)

As is clear from Equation (13), the larger the weld width W b , the smaller

the curvature radius R i is expected, with the same tilt angleθ .

Laser welded lap joints of the steels shown in Table 1 were subjected to tensile test, applied a tensile load to cause a sufficiently large rotational deformation, removed the load, and measured R

i and

θ through sectional observation. The relationship between these two is plotted in Fig. 8. The curves in the graph are the relationship between the two calculated from Equation (13). It is clear from the graph that the experimentally obtained relationship between R

i and

θ agrees well with that calculated from Equation (13), which represents the geometric demand.

Next, it is necessary to calculate the relationship of the tensile load T with the curvature radius R

i or the tilt angleθ. Furusako et al. used

the dimensionless parameterβ for the tensile load and conducted regression analysis as follows3):

Ri = 147.84 − 147.93β Ws

Lb W b 0.2 (14)

Here, it is impossible to obtainθ in the form of a function of R i

from Equation (13), and it will be rather troublesome to determine θwith respect to the value of R

i determined from Equation (14). In

consideration of this, we attempted to directly determineθ as a function of the dimensionless parameterβ , and determined the coefficient α using the equation below through a regression analysis.

θ = α β 1.5

TS MPa 1.25 (15)

Fig. 9 shows the relationship between the actually measured tilt angle θ shown in Fig. 8 and the regression estimate, obtained assuming that the value ofα in Equation (15) is 45,000. One can see that the two are in reasonably good agreement. 3.1.5 Mechanical properties of portion R

Because the portion R includes a heat affected zone (hereinafter written as HAZ) caused by welding, its mechanical properties are inhomogeneous. The mechanical properties of HAZ are similar to those of the weld metal at a position adjacent to weld metal, and as the distance from the weld metal increases, they gradually change

and become those of the base metal. As shown in Fig. 4, the fracture at the portion R does not occur close to the interface with the weld metal but at a position a little away from it because of weld metal’s restriction on the plastic deformation of the portion R. In consideration of this, it was presumed that the mechanical properties of the fractured part were the average of those of the base metal and weld metal. Thus, the tensile strength TS

R and uniform elongation

UE R of the portion R were supposed, respectively, as follows:

TSR = TSBM + TSWM / 2 (16)

UER = UEBM + UEWM / 2 (17)

Here, TS BM

and UE WM

are measured values. When the tensile strength and uniform elongation of the portion

R are given, then the modulus of longitudinal elasticity F and work hardening coefficient n are obtained using the following equations, and it becomes possible to use Equation (6) expressing the relationship between the stress and the strain in the portion R.

F = TSR ⋅ e / n n (18)

n = ln 1 + UER (19)

Here, e is the base of natural logarithm. 3.2 Estimation of fracture position and joint strength

The following summarizes what has been described above. Two steel sheets, t in thickness and W

s in width each, are lap welded

together by laser to form a bead W b in width and L

b in length, and this

joint is subjected to tensile shear test. Using a dimensionless parameterβ (β = 0 to 1), one can estimate the state of stress and the conditions for fracture at different portions of a joint under a tensile load as described below.

Letting the tensile strength of the base metal be TS BM

, from Equation (2), the stressσ

B in the base metal portion is:

σ B β = β ⋅ TSBM (20)

The base metal fractures whenβ = 1, and at that time,σ B satisfies

the following equation:

σ B 1 = TSBM (21)Fig. 8 Relationship between curvature radius R i and tilt angleθθθθθ in

tensile shear test

Fig. 9 Regression analysis of specimen tilt angle in tensile shear test

NIPPON STEEL TECHNICAL REPORT No. 95 January 2007

- 33 -

Fig. 10 Estimation procedure for fracture portion and maximum load

When the modulus of longitudinal elasticity F, work hardening coefficient n and tensile strength TS

R of the portion R are obtained

using Equations (16) to (19), the stress at the outer surface of the portion R can be determined by Equation (22) below, which is obtained from Equation (9).

σ R β = F ⋅ t / 2 + a β

Ri β + t / 2 − a β

n

(22)

Then, the tilt angleθ of the weld joint is calculated from Equation (15) as a function ofβ, and the curvature radius R

i at the inner surface

of the portion R (see Fig. 5) from Equation (13), thus:

θ β = α β 1.5

Lb / Ws 1.5

Wb / t 1.0

2 − Wb

1 − cos θ β (24)

On the other hand, the value of a is determined using Equation (25) below, which is given by substituting Equations (3) and (5) in Equation (8).

β = Lb ⋅ F

n

2 n + 1 (25)

Inconveniently, a is not explicitly expressed as a function ofβ, but the value of a that satisfies Equation (25) can be obtained comparatively easily by using a spreadsheet.

The condition for fracture at the portion R is given as follows:

σ R β = TSR (26)

The shear stress in the weld metal is, from Equation (11),

τ β = β ⋅ TSBM ⋅ Ws ⋅ t

Lb ⋅ Wb cos θ β (27)

Letting the hardness of the weld metal be Hv WM

, the condition for fracture at the weld metal is given by Equation (12) as follows:

τ β = 1.9 ⋅ HvWM (28)

To obtain the load T at the time of failure from the dimensionless parameterβ, the following equation is used based on Equation (3):

T β = β ⋅ TSBM ⋅ Ws ⋅ t (29)

When the test piece width W s , weld length L

b and weld width W

b are

given, the procedures for estimating the maximum tensile shear load that a laser welded lap joint can withstand and the position of fracture are as described below.

Fig. 10 shows an example of the estimation of the fracture position and load of test pieces, each made of mild steel sheets, 1.0 mm in thickness and 50 mm in width, lap welded by laser to form a weld bead 40 mm in length. The estimation was made on three different cases of weld widths: 0.5, 1.0 and 2.0 mm. The values of the variables necessary for the calculation are given in the graphs.

Increasing the value ofβ from 0 to 1 is the same as increasing the load in the tensile test. After determining the value ofβ , the stresses in the base metal and the outer surface of the portion R, and the shear stress in the weld metal are calculated using Equations (20),

(22), and (27), respectively. Increasing the value ofβ gradually, and when the above stress value for each of the portions becomes equal to the values representing the failure conditions given by Equations (21), (26), or (28) at any one of them, then the joint is expected to fail at that portion. The joint strength at that time is given by substituting the value ofβ in Equation (29).

As Fig. 10 shows, when the weld width is as small as 0.5 mm, then the shear stressτ of the weld metal exceedsτ

max even with

the smallest value ofβ, the test piece is expected to fracture at weld metal, and the value ofβ , namely the joint efficiency, is approximately 0.47. When the weld width is doubled to 1 mm, the shear stressτof weld metal decreases accordingly, but the stress in the outer surface of the portion R does not decrease as much, and as a result, the test piece is expected to fail at the portion R, with an joint efficiencyβ= 0.89. When the weld width is as large as 2 mm, on the other hand, the value ofβreaches 1.0 before the stress in the weld metal or portion R increases to the fracture limit, and the joint is expected to fail at the base metal. 3.3 Comparison of estimation results with test results

The authors verified how well the above method for estimating the fracture position and joint strength would reproduce test results. Test pieces were prepared by welding mild steel sheets 0.8, 1.0 and 1.2 mm in thickness and 40 and 50 mm in width by laser lap welding, and subjected these joints to tensile shear test. The results are plotted in Fig. 11; different plotting marks correspond to different fracture

NIPPON STEEL TECHNICAL REPORT No. 95 January 2007

- 34 -

Fig. 11 Effect of weld length and weld width on fracture portion and joint strength in tensile shear test

positions and the figures between parentheses indicate the joint efficiency actually measured. The fracture position and joint strength were also estimated using the values shown in Fig. 10. It is understood from Fig. 10 that, in the case where L

b / W

s = 0.8, a test piece is

expected to fail at the weld metal when W b /t = 0.5, and at the portion

R when W b / t = 1.0. Similar operations using different values of W

b /

t lead to an expectation that the fracture occurs at the weld metal when

W b / t is 0.85 or less, and at the portion R when W

b / t exceeds 0.85. The

above operations were repeated using different values of L b / W

s and

b / W

b / t where the weld metal

would fracture and those where the base metal would; the zones thus defined are also shown in Fig. 11. The curves in Fig. 11 show the relationship between L

b / W

b / t when the joint efficiencyβis

0.2, 0.4, 0.6, 0.8 and 1.0. Fig. 11 demonstrates that the developed estimation method is capable of qualitatively reproducing the fracture position and joint efficiency actually obtained through test. Thus, the estimation model summarized in Sub-section 3.2 is regarded as capable of explaining the fracture behavior of laser welded lap joints at tensile shear test.

4. Closing A model for estimating stresses in different portions of a laser

welded lap joint under a tensile shear load was developed, and the developed model proved capable of predicting the portion of fracture and the maximum withstand load of the weld joint. This attempt is expected to constitute a foundation for better understanding of the strength and fracture behavior of a laser welded lap, contributing to further enhancing the passenger safety of automobile bodies.

UDC 621 . 791 . 9 . 052 . 2 : 539 . 415

Tensile Shear Strength of Laser Welded Lap Joints Yasunobu MIYAZAKI*1 Seiji FURUSAKO*2

Abstract

The dependency of fracture position and maximum load of laser welded lap joints

on the weld-bead length and width was clarified through tensile shear test of joints,

and a mechanical prediction model for the test results was developed. Joints showed

the strength proportional to base metal tensile strength, which have the weld length

over 60% of specimen width or the weld width of 2 times of sheet thickness. The

developed model, which considers a joint dividing it into the base metal under uniaxial

tensile stress, a portion R under stretch bending and the weld metal under shear

stress, proved capable of qualitatively predicting the fracture behavior of laser welded

lap joints of mild steel sheets at tensile shear test.

1. Introduction Resistance spot welding has long been employed as a principal

welding method for assembling automobile bodies, but some carmakers, mainly in Europe, recently use laser welding in place of resistance spot welding1,2). Laser welding is a non-contact welding method and capable of joining materials by one-side access. While the European carmakers reportedly find laser welding economically advantageous because the electrode wear of spot welding can be avoided, they do not seem to fully enjoy the benefits of laser welding such as easy connection of hydro-forming parts and other closed- section components and higher joint strength due to continuous welding. A reason for this is presumably that the application of laser welding is generally limited to those portions where spot welding can be used as a backup in the case of a trouble with laser welding, and another is that the advantages of continuous welding by laser are not very clear.

Furthermore, unlike spot-welding joints, laser-welding joints are not axisymmetric, and many variables such as weld length, bead width and welding direction affect the strength of a joint of laser welding, and for this reason, the withstand load of a laser-welding joint has not been clear. In view of this, the authors already proposed a method for estimating the strength of laser welded lap joints3). In the present study, the authors partially reviewed the regression analysis employed for the estimation, and attempted to express the relationship between the size of a weld bead and joint strength in a simplified manner.

2. Shear Strength of Laser Welded Lap Joints 2.1 Experimental procedure

An experimental examination was conducted on the tensile shear strength of laser welded lap joints. Table 1 shows the mechanical properties of the steel sheets employed in this study; the sheet thickness was 1 mm and their tensile strength varied from 300 to 800 MPa. Fig. 1 schematically shows the test piece for the tensile shear test. An Nd-YAG laser having a work-piece power of 1.6 kW was used for welding the test pieces. To examine the effects of the bead size on joint strength, the weld length and width were changed by welding across the whole width of the test pieces or partially (weld lengths L

b of 50 and 30 mm, respectively) and setting the welding

speed at 1.6 and 0.7 m/min (weld widths W b of 0.85 and 2 mm,

respectively). Table 2 summarizes the welding conditions.

*1 Steel Research Laboratories *2 Nagoya R&D Lab.

Table 1 Mechanical properties of steels used

Steel

A

B

C

D

Thickness

(mm)

1

1

1

1

YP

(MPa)

142

339

392

435

TS

(MPa)

301

472

629

794

Elongation

- 29 -

The tensile shear test was conducted at room temperature and at a constant tension speed of 10 mm/min, and the maximum withstand load of each weld joint was measured. To examine the deformation of the test pieces, some of them were loaded to withstand load, the load was removed before failure, and the deformation around the weld joint was recorded through sectional observation. 2.2 Tensile test results

In the tensile shear test of laser welded lap joints, fracture occurred at the base metal (BM), weld metal (WM) or portion adjacent to the weld joint (herein referred to as the portion R). Fig. 2 shows the photographs of test pieces after fracture at different portions and schematic illustrations of the fracture portions, and Fig. 3 shows the relationship between the maximum load that the lap joints withstood before fracture (hereinafter written as the joint strength) and the strength of the base metal. The dotted line of the graph shows the product of the tensile strength (TS) and sectional area of the base metal, namely the maximum withstand load of a joint in the case of fracture at the base metal (hereinafter written as the base-metal strength insofar as it is not confused with the tensile strength of the base metal).

As Fig. 3 shows, when the weld width was 2.0 mm and the weld length was 50 mm across the whole width of the test piece, the fracture occurred at the base metal or portion R, and the joint strength was the same as the base-metal strength. In contrast, when the weld width was 0.85 mm and the weld length was 50 mm, the weld metal failed except for the test pieces of Steel A, the joint strength increased as the base-metal strength increased, and the joint strength did not decrease significantly below the base-metal strength. On the other hand, the test pieces of Steel A failed at the portion R, and the joint strength was equal to the base-metal strength.

When the bead width was 2.0 mm and its length was 30 mm, all the test pieces failed at portion R, and the joint strength increased as the base-metal strength increased. In contrast, when the bead width was 0.85 mm and the length was 30 mm, the weld metal failed except for the test pieces of Steel A, but different from the cases where the

weld length was 50 mm, the joint strength was nearly the same, not depending on the base-metal strength. The test pieces of Steel A failed at the portion R even though the bead width was as small as 0.85 mm. 2.3 Deformation under load

Part (a) of Fig. 4 shows a sectional view of a test piece deformed under a tensile load; the base metal is Steel A and the weld joint is 2.0 mm wide and 50 mm long. Before application of a tensile load, the thickness center planes of the two sheets were out of alignment from each other, but under a tensile load, the test piece underwent a torque about the weld metal. When the tensile load increased, the deformation increased such that the thickness center planes of the two sheets aligned with each other. On the other hand, the test piece shown in the lower frame of part (b) of Fig. 4, which had a weld width of 0.85 mm, failed at the weld metal before the thickness center planes of the two sheets were aligned with each other.

Fig. 1 Schematic diagram of laser lap joint for tensile shear test

Table 2 Welding conditions for tensile test specimens

Beam source

Focal position

Weld length L b (mm)

2kW Nd-YAG laser

0.7, 1.6

2, 0.85

30, 50

Fig. 2 Fracture mode of laser lap joint in tensile shear test

Fig. 3 Dependency of laser lap joint strength on tensile strength of steel

NIPPON STEEL TECHNICAL REPORT No. 95 January 2007

- 30 -

3. Mechanical Model of Stresses in Laser Welded Lap Joints under Tensile Shear Test Although it is possible to experimentally determine the strength

of joints having different weld lengths, weld widths and sheet widths, it is a tiresome and time-consuming business. In view of this, an attempt was made to construct a model to estimate the strength of a weld joint in consideration of the stress imposed on the joint by a tensile load. 3.1 Modeling of stresses at different portions of joint

The deformation of a joint shown in Fig. 4 (a) indicates that such a deformation can be studied dividing a joint under a tensile load into three portions: the weld metal, portion R and base metal shown in Fig. 5. The stress in each of these portions under a certain load can be estimated by studying it in a simple manner separated from that in the other portions. 3.1.1 Stress imposed on base metal

When the bead length and width are sufficiently large and the fracture occurs at a position away from the weld metal as shown in Fig. 2 (a), the base metal is considered to be under a uniaxial tensile stress just like a single-sheet test piece at tensile test. Under an outside force T, therefore, the stress imposed on the base metalσ

B can be

estimated using the following equation:

σB = T Ws ⋅ t (1)

where, W s is the width of the specimen, and t is its thickness.

We introduce a dimensionless parameterβ according to Equa- tion (2), which is the ratio between the stress on the base metalσ

B

:

β = σ B / TSBM (2)

Here, the value ofβ changes from 0 to 1, and the joint fails at the base metal when the stress increases toβ = 1.0.

Eliminating the stress σ B from Equations (1) and (2), the outside

force T can be expressed as follows using the dimensionless parameter β , which expresses the magnitude of the load:

T = β ⋅ TSBM ⋅ Ws ⋅ t (3)

3.1.2 Stress imposed on portion R Here, let us simplify the portion R as being in a tension bending

condition as shown in Fig. 6. This seems to be an adequate approximation as far as the center of the portion R is concerned,

Fig. 4 Deformation of lap joint under tensile shear load and configuration after fracture, through cross-section of joint

Fig. 5 Simplified model of joint and geometric demand for configu- ration

Fig. 6 Definition of parameters at portion R

NIPPON STEEL TECHNICAL REPORT No. 95 January 2007

- 31 -

excluding its interfaces with the base metal and weld metal. With respect to the case shown in the upper frame of Fig. 4 (b) where a joint fails at a position in the curved portion (portion R) a little away from the weld metal, this simplification would be adequate for a model for predicting the position of fracture.

Following a common analysis method of bending deformation, we suppose a neutral plane where there is no tension or compression: there is a compressive stress on the inner side of it and a tensile stress on the outer side.

Letting the curvature radius of the neutral plane be R e , the

circumferential strainε(r) at a plane away from the curvature center by a distance r is given as follows:

ε r = r ⋅ θ − Re ⋅ θ

Re ⋅ θ

= r − Re

Re

(4)

In addition, the relationship between the curvature radius R i of the

inner surface of the portion R, the curvature radius R e of the neutral

plane and the distance a between the neutral plane and the thickness center shown in Fig. 6 is given by the following equation:

Re = Ri + t / 2 − a (5)

Furthermore, using a relational expression frequently applied to the relationship between stress and strain, the relationship between the circumferential stressσ (r) and strainε (r) is given as follows:

σ r = F ⋅ εn r (6)

where, F is the modulus of longitudinal elasticity, or Young’s modulus, and n is a work hardening coefficient.

Based on the above and supposing that the integration of the circumferential stress in the portion R is equal to the tensile load T, the following equation can be obtained.

T = Lb σ r dr Ri

Ri + t

(7)

where, L b is the weld length. This integration is easily carried out by

using Equations (4), (5) and (6), and the following equation is obtained:

T = Lb ⋅ F n + 1

1 Re

(8)

Here, the thickness t was assumed not to change under the deformation.

The value ofσ (r) becomes largest at the outer surface, and the largest valueσ

R is given as follows:

σ R = F ⋅ t / 2 + a Ri + t / 2 − a

n

(9)

A joint is expected to fail at the portion R when the value ofσ R reaches

the tensile strength TS R determined by the material quality of the portion

R. 3.1.3 Stress imposed on weld metal

In the case where a joint fails at the weld metal, as shown in Fig. 4 (b), the weld metal fails by shear fracture without significant deformation. The average shear stressτimposed on the weld metal under a tensile load T is expressed by Equation (10) below.

τ = T cos θ Lb ⋅ Wb

(10)

Lb ⋅ Wb cos θ (11)

where, θis the tilt angle of the weld joint resulting from the tensile load shown in Fig. 7, and W

b is the weld width as measured between

the two sheets. The dimensionless parameterβ , which expresses the magnitude of the load in Equation (3), was used for the modification from Equation (10) to Equation (11).

While shear stress is estimated at 1 / 3 times tensile strength, tensile strength TS is known to be in good correlation with Vickers hardness Hv, and when stress is expressed in terms of MPa, the relationship between these two is expressed as TS = Hv/3× 9.8. Therefore, when the hardness of weld metal Hv

WM is given, it is

possible to estimate the maximum shear stress τ max

that the weld metal can withstand by the following equation:

τ max = TSWM / 3

(12)

A joint is expected to fail by shear fracture of weld metal when the shear stressτgiven by Equation (11) becomes equal to the maximum shear stressτ

max given by Equation (12).

To estimate the shear stressτ imposed on weld metal based on Equation (11), however, it is necessary to know the tilt angleθ . 3.1.4 Relationship between tensile load and tilt angle of test piece

Let us suppose that, in Fig. 5, the weld metal, portion R and base metal connect to each other smoothly, that is, the boundary lines between the portion R and base metal are perpendicular to the direction of the tensile load. Here, it is easy to calculate the vector a from the weld center C to the thickness center X on the boundary line between the portion R and base metal and the vector b from the curvature center O of the portion R to the point X. These two vectors are perpendicular to each other when the deformation is well advanced and the thickness centers of the two sheets are aligned with each other. This geometrical demand is expressed as follows using the vector c from the curvature center O to the weld center C:

a ⋅ b = b − c ⋅ b

= Ri + t 2 ⋅ 1 − cos θ ⋅ Ri + t

2 + Wb

= 0

Since R i t / 2 is positive, the following equation is obtained:

Fig. 7 Stress state at each part of joint

NIPPON STEEL TECHNICAL REPORT No. 95 January 2007

- 32 -

2 − Wb

1 − cos θ (13)

As is clear from Equation (13), the larger the weld width W b , the smaller

the curvature radius R i is expected, with the same tilt angleθ .

Laser welded lap joints of the steels shown in Table 1 were subjected to tensile test, applied a tensile load to cause a sufficiently large rotational deformation, removed the load, and measured R

i and

θ through sectional observation. The relationship between these two is plotted in Fig. 8. The curves in the graph are the relationship between the two calculated from Equation (13). It is clear from the graph that the experimentally obtained relationship between R

i and

θ agrees well with that calculated from Equation (13), which represents the geometric demand.

Next, it is necessary to calculate the relationship of the tensile load T with the curvature radius R

i or the tilt angleθ. Furusako et al. used

the dimensionless parameterβ for the tensile load and conducted regression analysis as follows3):

Ri = 147.84 − 147.93β Ws

Lb W b 0.2 (14)

Here, it is impossible to obtainθ in the form of a function of R i

from Equation (13), and it will be rather troublesome to determine θwith respect to the value of R

i determined from Equation (14). In

consideration of this, we attempted to directly determineθ as a function of the dimensionless parameterβ , and determined the coefficient α using the equation below through a regression analysis.

θ = α β 1.5

TS MPa 1.25 (15)

Fig. 9 shows the relationship between the actually measured tilt angle θ shown in Fig. 8 and the regression estimate, obtained assuming that the value ofα in Equation (15) is 45,000. One can see that the two are in reasonably good agreement. 3.1.5 Mechanical properties of portion R

Because the portion R includes a heat affected zone (hereinafter written as HAZ) caused by welding, its mechanical properties are inhomogeneous. The mechanical properties of HAZ are similar to those of the weld metal at a position adjacent to weld metal, and as the distance from the weld metal increases, they gradually change

and become those of the base metal. As shown in Fig. 4, the fracture at the portion R does not occur close to the interface with the weld metal but at a position a little away from it because of weld metal’s restriction on the plastic deformation of the portion R. In consideration of this, it was presumed that the mechanical properties of the fractured part were the average of those of the base metal and weld metal. Thus, the tensile strength TS

R and uniform elongation

UE R of the portion R were supposed, respectively, as follows:

TSR = TSBM + TSWM / 2 (16)

UER = UEBM + UEWM / 2 (17)

Here, TS BM

and UE WM

are measured values. When the tensile strength and uniform elongation of the portion

R are given, then the modulus of longitudinal elasticity F and work hardening coefficient n are obtained using the following equations, and it becomes possible to use Equation (6) expressing the relationship between the stress and the strain in the portion R.

F = TSR ⋅ e / n n (18)

n = ln 1 + UER (19)

Here, e is the base of natural logarithm. 3.2 Estimation of fracture position and joint strength

The following summarizes what has been described above. Two steel sheets, t in thickness and W

s in width each, are lap welded

together by laser to form a bead W b in width and L

b in length, and this

joint is subjected to tensile shear test. Using a dimensionless parameterβ (β = 0 to 1), one can estimate the state of stress and the conditions for fracture at different portions of a joint under a tensile load as described below.

Letting the tensile strength of the base metal be TS BM

, from Equation (2), the stressσ

B in the base metal portion is:

σ B β = β ⋅ TSBM (20)

The base metal fractures whenβ = 1, and at that time,σ B satisfies

the following equation:

σ B 1 = TSBM (21)Fig. 8 Relationship between curvature radius R i and tilt angleθθθθθ in

tensile shear test

Fig. 9 Regression analysis of specimen tilt angle in tensile shear test

NIPPON STEEL TECHNICAL REPORT No. 95 January 2007

- 33 -

Fig. 10 Estimation procedure for fracture portion and maximum load

When the modulus of longitudinal elasticity F, work hardening coefficient n and tensile strength TS

R of the portion R are obtained

using Equations (16) to (19), the stress at the outer surface of the portion R can be determined by Equation (22) below, which is obtained from Equation (9).

σ R β = F ⋅ t / 2 + a β

Ri β + t / 2 − a β

n

(22)

Then, the tilt angleθ of the weld joint is calculated from Equation (15) as a function ofβ, and the curvature radius R

i at the inner surface

of the portion R (see Fig. 5) from Equation (13), thus:

θ β = α β 1.5

Lb / Ws 1.5

Wb / t 1.0

2 − Wb

1 − cos θ β (24)

On the other hand, the value of a is determined using Equation (25) below, which is given by substituting Equations (3) and (5) in Equation (8).

β = Lb ⋅ F

n

2 n + 1 (25)

Inconveniently, a is not explicitly expressed as a function ofβ, but the value of a that satisfies Equation (25) can be obtained comparatively easily by using a spreadsheet.

The condition for fracture at the portion R is given as follows:

σ R β = TSR (26)

The shear stress in the weld metal is, from Equation (11),

τ β = β ⋅ TSBM ⋅ Ws ⋅ t

Lb ⋅ Wb cos θ β (27)

Letting the hardness of the weld metal be Hv WM

, the condition for fracture at the weld metal is given by Equation (12) as follows:

τ β = 1.9 ⋅ HvWM (28)

To obtain the load T at the time of failure from the dimensionless parameterβ, the following equation is used based on Equation (3):

T β = β ⋅ TSBM ⋅ Ws ⋅ t (29)

When the test piece width W s , weld length L

b and weld width W

b are

given, the procedures for estimating the maximum tensile shear load that a laser welded lap joint can withstand and the position of fracture are as described below.

Fig. 10 shows an example of the estimation of the fracture position and load of test pieces, each made of mild steel sheets, 1.0 mm in thickness and 50 mm in width, lap welded by laser to form a weld bead 40 mm in length. The estimation was made on three different cases of weld widths: 0.5, 1.0 and 2.0 mm. The values of the variables necessary for the calculation are given in the graphs.

Increasing the value ofβ from 0 to 1 is the same as increasing the load in the tensile test. After determining the value ofβ , the stresses in the base metal and the outer surface of the portion R, and the shear stress in the weld metal are calculated using Equations (20),

(22), and (27), respectively. Increasing the value ofβ gradually, and when the above stress value for each of the portions becomes equal to the values representing the failure conditions given by Equations (21), (26), or (28) at any one of them, then the joint is expected to fail at that portion. The joint strength at that time is given by substituting the value ofβ in Equation (29).

As Fig. 10 shows, when the weld width is as small as 0.5 mm, then the shear stressτ of the weld metal exceedsτ

max even with

the smallest value ofβ, the test piece is expected to fracture at weld metal, and the value ofβ , namely the joint efficiency, is approximately 0.47. When the weld width is doubled to 1 mm, the shear stressτof weld metal decreases accordingly, but the stress in the outer surface of the portion R does not decrease as much, and as a result, the test piece is expected to fail at the portion R, with an joint efficiencyβ= 0.89. When the weld width is as large as 2 mm, on the other hand, the value ofβreaches 1.0 before the stress in the weld metal or portion R increases to the fracture limit, and the joint is expected to fail at the base metal. 3.3 Comparison of estimation results with test results

The authors verified how well the above method for estimating the fracture position and joint strength would reproduce test results. Test pieces were prepared by welding mild steel sheets 0.8, 1.0 and 1.2 mm in thickness and 40 and 50 mm in width by laser lap welding, and subjected these joints to tensile shear test. The results are plotted in Fig. 11; different plotting marks correspond to different fracture

NIPPON STEEL TECHNICAL REPORT No. 95 January 2007

- 34 -

Fig. 11 Effect of weld length and weld width on fracture portion and joint strength in tensile shear test

positions and the figures between parentheses indicate the joint efficiency actually measured. The fracture position and joint strength were also estimated using the values shown in Fig. 10. It is understood from Fig. 10 that, in the case where L

b / W

s = 0.8, a test piece is

expected to fail at the weld metal when W b /t = 0.5, and at the portion

R when W b / t = 1.0. Similar operations using different values of W

b /

t lead to an expectation that the fracture occurs at the weld metal when

W b / t is 0.85 or less, and at the portion R when W

b / t exceeds 0.85. The

above operations were repeated using different values of L b / W

s and

b / W

b / t where the weld metal

would fracture and those where the base metal would; the zones thus defined are also shown in Fig. 11. The curves in Fig. 11 show the relationship between L

b / W

b / t when the joint efficiencyβis

0.2, 0.4, 0.6, 0.8 and 1.0. Fig. 11 demonstrates that the developed estimation method is capable of qualitatively reproducing the fracture position and joint efficiency actually obtained through test. Thus, the estimation model summarized in Sub-section 3.2 is regarded as capable of explaining the fracture behavior of laser welded lap joints at tensile shear test.

4. Closing A model for estimating stresses in different portions of a laser

welded lap joint under a tensile shear load was developed, and the developed model proved capable of predicting the portion of fracture and the maximum withstand load of the weld joint. This attempt is expected to constitute a foundation for better understanding of the strength and fracture behavior of a laser welded lap, contributing to further enhancing the passenger safety of automobile bodies.

Recommended